define the correct loading curves: pressure vs. time and axial feed vs. time. In the case of more complex tube hydroformed parts the tube must be pre-bent prior to loading into the hydroforming die. Bending is done sequentially along the length of the tube, with the tube being bent around bending discs (or dies) as the tube length is fed in. Bending can be done with or without mandrels. This additional complexity of process further increases the reliance on FEM for designing and evaluating manufacturing processes. The feasibility of a hydroforming process must take into consideration the initial tube material properties and its potential for variation, along with the bending process, hydraulic pressure throughout the forming process, in inclusion of axial feed or not, in order to predict metal formability. Typical tools Tools and punches can be interchanged for different part requirements. One advantage of hydroforming is the savings on tools. For sheet metal only a draw ring and punch (metalworking) or male die is required. Depending on the part being formed, the punch can be made from epoxy, rather than metal. The bladder of the hydroform itself acts as the female die eliminating the need to fabricate it. This allows for changes in material thickness to be made with usually no necessary changes to the tool. However, dies must be highly polished and in tube hydroforming a two-piece die is required to allow opening and closing. Geometry produced Another advantage of hydroforming is that complex shapes can be made in one step. In sheet hydroforming with the bladder acting as the male die almost limitless geometries can be produced. However, the process is limited by the very high closing force required in order to seal the dies, especially for large panels and thick hard materials. Small concave corner radii are difficult to be completely calibrated, i.e. filled, because too large a pressure would be required. in fact, the die closing force can be very high, both in tube and sheet hydroforming and may easily overcome the maximum tonnage of the forming press. In order to keep the die closing force under prescribed limits, the maximum internal fluid pressure must be limited. This reduces the calibration abilities of the process, i.e. it reduces the possibility of forming parts with small concave radii. Limits of the sheet hydroforming process are due to risks of excessive thinning, fracture, wrinkling and are strictly